Presentation on theme: "Viscoelastic properties Polymers have both ideal elastic and viscous behavior depending on time and temperature."— Presentation transcript:
Viscoelastic properties Polymers have both ideal elastic and viscous behavior depending on time and temperature.
Ideal (elastic) Solid Hooks Law response is independent of time and the deformation is dependent on the spring constant.
Ideal Liquid = viscosity de/dt = strain rate The viscous response is generally time- and rate-dependent.
The behaviour of linear elastic were given by Hooke’s law: E = Elastic modulus = Stress e= strain de/dt = strain rate d /dt = stress rate = viscosity or The behaviour of linear viscous were given by Newton’s Law: ** This equation only applicable at low strain
Behaviour of most polymer is in between behaviour of elastic and viscous materials. 1. At low temperature & high strain rate, Polymer demonstrate elastic behaviour, 2. At high temperature & low strain rate, Polymer demonstrate viscous behaviour 3. At intermediate temperatures & rate of strain Polymer demonstrate visco-elastic behaviour Viscoelastic behavior
Polymer is called visco- elastic because: Showing both behaviour elastic & viscous behaviour Instantaneously elastic strain followed by viscous time dependent strain Load added Load released elastic viscous
Kelvin Voigt Model
Static Modulus of Amorphous PS Glassy Leathery Rubbery Viscous Polystyrene Stress applied at x and removed at y
Dynamic Mechanical Analysis
Spring Model = 0 ⋅ sin (ω ⋅ t) maximum strain = angular velocity Since stress, is G G sin t And and are in phase
Dashpot Model Whenever the strain in a dashpot is at its maximum, the rate of change of the strain is zero ( = 0). Whenever the strain changes from positive values to negative ones and then passes through zero, the rate of strain change is highest and this leads to the maximum resulting stress.
Dynamic (Oscillatory) Testing In the general case when the sample is deformed sinusoidally, as a response the stress will also oscillate sinusoidally at the same frequency, but in general will be shifted by a phase angle with respect to the strain wave. The phase angle will depend on the nature of the material (viscous, elastic or viscoelastic) Input Response where 0°< <90° 3.29 stress strain viscosityG modulus
Dynamic (Oscillatory) Testing By using trigonometry: Let’s define: In-phase component of the stress, representing solid- like behavior Out-of-phase component of the stress, representing liquid-like behavior where: (3-1) 3.30
Physical Meaning of G ’, G ” Equation (3-1) becomes: We can also define the loss tangent: For solid-like response: For liquid-like response: G’ storage modulusG’’ loss modulus
Real Visco-Elastic Samples
Typical Oscillatory Data Rubbers – Viscoelastic solid response: G’ > G” over the whole range of frequencies G’ G’’ log G log Rubber G’ storage modulus G’’ loss modulus
Typical Oscillatory Data Polymeric liquids (solutions or melts) Viscoelastic liquid response: G” > G’ at low frequencies Response becomes solid-like at high frequencies G’ shows a plateau modulus and decreases with -2 in the limit of low frequency (terminal region) G” decreases with -1 in the limit of low frequency G’ G’’ log G log Melt or solution G0G0 G’ storage modulus G’’ loss modulus Less liquid like More liquid like
Polyurethane foam (Tg 160 C) G’ storage modulus G’’ loss modulus
These data show the difference between the behaviour of un-aged and aged samples of rubber, and were collected in shear mode on the DMTA at 1 Hz. The aged sample has a lower modulus than the un-aged, and is weaker. The loss peak is also much smaller for the aged sample. G’ storage modulus G’’ loss modulus